Progress In Electromagnetics Research Letters, Vol. 60, 73–80, 2016

Microwave Characterization of Electrical Conductivity of Composite Conductors by Half-Wavelength Coplanar Resonator Bilal Benarabi1, * , Faouzi Kahlouche1 , Bernard Bayard1 , Anthony Chavanne2 , and Jeremy Sautel3

Abstract—The aim of this work is to characterize the electrical conductivity of composite conductors deposited on an alumina substrate. Several half-wavelength coplanar resonators are realized using several pure conductors, silver (Ag), copper (Cu), gold (Au) and tin (Sn), to compare their quality factors (Q0 ), related to losses, with those from analytical methods. In the literature, losses in coplanar components have been estimated by diﬀerent analytical methods. We have put in evidence the relationship between electrical conductivity of the conductor and the resonator quality factor. An overall good agreement among quality factor values obtained by the analytical formulas, by numerical simulations and by microwave measurements is observed. The surface roughness is taken into account to better estimate real conductor losses. Therefore, these analytical formulas are used to extract the electrical conductivity values of the composite conductors (Ag-aC, AgSnIn and AgSn), from measured quality factors.

1. INTRODUCTION This work is part of a research project (Plug In Nano) whose objective is to oﬀer a new composite conductor, instead of gold used as a coating conductor in microwave and automotive connectors. The new composite conductors developed during this project have unknown electrical conductivities. In the literature, little work has been done on the characterization of the eﬀective electrical conductivity of materials [1, 2]. Our characterization method makes use of the relationship between the resonator quality factor (Q0 ) and associated losses (αT ), which depends, among several parameters, on the electrical conductivity of the metal which forms the resonator. Several analytical formulas for the estimation of these losses, in coplanar components (CPW), have been developed [3, 4]. First, we have veriﬁed experimentally and numerically these formulas by microwave measurements of losses and quality factor Q0 of half-wavelength resonators realized by some known conductors such as silver (Ag), copper (Cu), gold (Au) and tin (Sn). Then, we have extracted the electrical conductivities values of the composite conductors from measured quality factors of resonators realized with these metals. Three new composite conductors are measured here, which are: silveramorphous carbon (Ag-aC), silver-tin-indium (AgSnIn) and silver-tin (AgSn). 2. ANALYTICAL FORMULAS OF LOSSES Three loss sources are considered in coplanar half-wavelength (λ/2) resonator, as shown in Figure 1: - Conductor loss (αc ); because of the ﬁnite conductivity of the conductor. Received 4 March 2016, Accepted 10 April 2016, Scheduled 20 May 2016 * Corresponding author: Bilal Benarabi ([email protected]). 1 Laboratoire Hubert Curien, UMR CNRS 5516, 18 rue Benoˆ ıt Lauras, St-Etienne 42000, France. Bouth´eon Cedex, France. 3 Radiall-Centr’Alp, 642 rue E. Romanet, Voreppe 38340, France.

2

IREIS, ZI Sud, Andr´ ezieux-

74

Benarabi et al.

W

S

W

Resonant line (λ/2)

ε0 t

h

Figure 1. λ/2 CPW resonator.

ε 0 εr

Figure 2. CPW line dimensions.

- Dielectric loss (αd ); due to the heating eﬀects in the dielectric. - Radiation loss (αr ); which can be split into surface wave and space wave components. 2.1. Dielectric Loss For CPW line, the attenuation due to dielectric losses in the substrate is [5]: π εr αd = q tan δ [Np/m] √ λ0 εeﬀ

(1)

tan δ is the dielectric loss tangent and εeﬀ the eﬀective permittivity of the CPW, εeﬀ = 1 + q (εr − 1)

(2)

1 K(k1 ) K(k0 ) 2 K(k1 ) K(k0 )

(3)

q is the ﬁlling factor, q=

The terms K (k1 ) and K (k0 ) are the complete elliptic integrals of the ﬁrst kind with moduli k0 and k1 , which are given by: sinh(πS/4h) π(S + 2W ) sinh 4h S k0 = S + 2W are the complementary moduli given by 2 = 1 − k0,1 k0,1 k1 =

The terms k0,1

(4)

(5)

(6)

S, W and h are the geometric parameters of the structure (Figure 2). 2.2. Conductor Loss The attenuation constant αc due to conductor loss in the center strip conductor and the ground planes of the CPW is investigated by several methods. - In the Conformal Mapping method [5], the expression of attenuation constant αc is given below. The assumption made in deriving this expression is that thickness t of the CPW conductors is far greater than the skin depth δ in the metal. Typically, t is greater than 5δ. Rc + Rg [Np/m] (7) 2Z0 where Rc is the series resistance in ohms per unit length of the center strip conductor and is given by: 4πS Rs 1 + k0 π + ln − k0 ln (8) Rc = t 1 − k0 4S 1 − k02 K 2 (k0 ) αc =

Progress In Electromagnetics Research Letters, Vol. 60, 2016

75

Rg is the distributed series resistance in ohms per unit length of the ground planes and is given by: k0 Rs 1 + k0 4π(S + 2W ) 1 ln π + ln − (9) Rg = t k0 1 − k0 4S 1 − k02 K 2 (k0 ) and Z0 is the coplanar waveguide characteristic impedance. The term Rs is the skin eﬀect surface resistance given by: 1 Rs = [Ohms] (10) σδ where σ is the conductivity of the conductor in Siemens/meter and δ the skin depth. - Ghione and Naldi [6] obtained the expression for the conductor loss through an extension of Owyang an Wu’s conformal mapping approach [7]:

√ Rs εeﬀ 8πa(1 − k0 ) 1 8πb(1 − k0 ) 1 π + log − π + log (11) αc = a t(1 + k0 ) b t(1 + k0 ) 480πK(k0 )K (k0 ) 1 − k02 - In Matched Asymptotic technique [8], both the ﬁnite thickness and non-ideal conductivity of the CPW conductors are taken into account to calculate the conductor loss. In addition, the shape of the conductor cross-section need not be rectangular, but instead can be trapezoidal. Thus, the sides of the conductor which are normally assumed to be vertical can now be considered to be inclined at an angle θ as shown in Figure 3. In the same ﬁgure, the average center strip width and ground plane separation are indicated as 2a and 2b, respectively.

Figure 3. Coplanar waveguide conductor geometry showing the stopping distance Δ and edge proﬁle θ. The attenuation constant αc due to conductor loss is given by

1 2a (b − a) 1 2b (b − a) Rsm b2 ln + ln (12) αc = 16Z0 [K 2 (k)] (b2 − a2 ) a Δ (b + a) b Δ (b + a) where a (13) k = b cot(kc t) + csc(kc t) (14) Rsm = ωμ0 tIm kc t 2π σ −j (15) kc = λ0 ωε0 The stopping distance Δ for a given conductor thickness t, skin depth δ and edge proﬁle θ is given in Table 1 in [8]. 2.3. Radiation Loss In addition to the conductor and dielectric losses, the loss of the energy radiated in the coplanar line contributes signiﬁcantly to the total losses. It strongly depends on the frequency and geometry of the structure. For thick substrates, radiation losses are dominant because the CPW radiates much in the dielectric. The attenuation constant αrd due to radiation loss is given by [9]: π 5 1 (1 − 1/ε )2 (S + 2W )2 ε3/2 r r √ f3 (16) αrd = 3 2 2 1 + 1/εr c K (k)K(k)

76

Benarabi et al.

k = k0 given in Equation (5), and f is the frequency. Equation (16) is supposed to be valid under the conditions of geometry (Figure 2) limited by 0.1 < S/W < 10, thickness of the substrate h > 3W and wavelength λ > S + 2W . Total losses (αT ) which are the sum of all these components are related to the resonator unloaded quality factor Q0 by the following formula [10]: √ π εeﬀ Q0 = (17) λ0 αT λ0 , εeﬀ are the free space wavelength and eﬀective permittivity, respectively, which are related to the length of the cavity resonator (l) by [5]: λ0 (18) l= √ 2 εeﬀ The Q0 factor is calculated from the load quality factor QL at resonance by: Q0 = where QL =

QL 1 − 10(−LA /20)

(19)

f0 f2–3 dB − f1–3 dB

(20)

LA is the insertion loss at resonance. f0 and f1–3 dB , f2–3 dB are, respectively, the resonant frequency and the frequencies at −3 dB. 3. REALIZATION AND MEASUREMENT The components are manufactured by the following steps. The 4 µm conductor layer is obtained by electro-deposition and chemical formulation of metal on an alumina substrate (Al2 O3 ) with a relative dielectric permittivity of 9.8 and dielectric loss tangent of 10−4 . The samples are then passed to the photolithography step and etching by an etchant which depends on the metal: ferric chloride for copper, nitric acid for silver and nickel, and cyanuric acid for gold (Figure 4). Composite conductors are etched by femtosecond laser technique (Figure 5). Three λ/2 resonators have been designed and produced following the steps mentioned above, with dimensions and resonant frequencies given in Table 1.

Figure 4. Realized CPW resonators on alumina substrate with pure conductors: Ag, Cu, Au and Sn (4 µm).

Figure 5. Realized CPW resonators on alumina substrate with composite conductors, to be characterized: Ag-aC, AgSnIn and AgSn (4 µm).

Progress In Electromagnetics Research Letters, Vol. 60, 2016

77

Table 1. Dimensions of fabricated λ/2 resonators. λ/2 resonator Length (l = λ/2) Frequency (f0 )

S = 330 µm 10.6 mm 6 GHz

W = 146 µm 6.3 mm 4.2 mm 10 GHz 15 GHz

The loaded Q factor (QL ) is calculated by Equation (24) where the frequencies are determined from S12 and S21 transmission coeﬃcients measured by a vector network analyzer (VNA) through coplanar probes after calibration with an adapted kit in the frequency band [10 MHz–25 GHz]. In the HFSS software, resonators were excited through two wave ports, and an absorbing boundary condition was applied in the air box to simulate radiation losses. We used the same dielectric substrate and diﬀerent values of ﬁnite conductivity that corresponds to the pure conductors. 4. RESULTS AND DISCUSSION Tables 2, 3 and 4 show the evolution of the unloaded quality factor of resonators realized with pure conductors: silver (Ag), copper (Cu), gold (Au) and tin (Sn), as a function of their electrical conductivities, with respectively the following values: 61, 58, 41 and 9 MS/m. According to losses formulas, dielectric and radiation losses are supposed to be constant for the same design structure, and only the conductor loss changes when the metal is altered. The results show the variation of the resonator quality factor (Q0 ) as a function of the electrical conductivity of the conductor which put in evidence the relationship between these parameters. We observe an overall good correlation between the Q0 factors obtained by the analytical formulas, numerical simulation of HFSS and by microwave measurement of the three resonators with a small diﬀerence in some points where the Q0 factor of theory and numerical simulation is a bit larger than Table 2. Experimental, numerical and analytical Q0 factors values of CPW λ/2 resonators realized by pure conductors, Ag, Cu, Au and Sn, with f0 = 6 GHz. Quality factors values (Q0 ) of CPW λ/2 resonator with f0 = 6 GHz Q0 Mean value Purs Mapping Mapping Asymptotic HFSS Measured and uncertainty conductors (G. Ghione) Ag 142.99 152.03 144.13 142.58 139.95 144.33 ± 2.7 Cu 140.33 149.58 141.46 132.6 128.36 138.46 ± 4.7 Au 87.23 93.17 88.18 84.69 85.55 87.76 ± 1.9 Sn 39.53 21.8 40.06 28.45 28.01 31.57 ± 4.1 Table 3. Experimental, numerical and analytical Q0 factors values of CPW λ/2 resonators realized by pure conductors, Ag, Cu, Au and Sn, with f0 = 10 GHz. Quality factors values (Q0 ) of CPW λ/2 resonator with f0 = 10 GHz Q0 Mean value Purs Mapping Mapping Asymptotic HFSS Measured and uncertainty conductors (G. Ghione) Ag 132.28 130.81 132.63 128.3 123.15 129.34 ± 2.1 Cu 130.71 129.27 131.08 126.09 118.01 127.03 ± 2.9 Au 92.84 94.66 93.45 88.06 93.55 92.51 ± 1.47 Sn 46.95 50.38 47.47 45.03 39.98 45.96 ± 2.3

78

Benarabi et al.

Table 4. Experimental, numerical and analytical Q0 factors values of CPW λ/2 resonators realized by pure conductors, Ag, Cu, Au and Sn, with f0 = 15 GHz. Quality factors values (Q0 ) of CPW λ/2 resonator with f0 = 15 GHz Q0 Mean value Purs Mapping Mapping Asymptotic HFSS Measured and uncertainty conductors (G. Ghione) Ag 116.56 115.92 115.86 125.3 122.07 119.42 ± 2.1 Cu 115.37 114.71 114.71 115.09 113.44 114.66 ± 0.4 Au 82.68 83.06 82.69 79.56 76.41 80.88 ± 1.5 Sn 31.12 24.53 31.42 28.03 21.66 27.35 ± 2.2 Table 5. Measured Q0 factors of λ/2 resonators with f0 = 6, 10 and 15 GHz, realized by composite conductors. Composite conductors Q0 factors (f0 = 6 GHz) Q0 factors (f0 = 10 GHz) Q0 factors (f0 = 15 GHz)

Ag-aC 100.39 105.6 89.3

AgSnIn 57.94 67.92 64.95

AgSn 49.7 56.43

measured one. The surface roughness of conductors increases the conductor losses (αc ). We have used Hammerstad and Bekkadal formula [11], to take into account the eﬀects of surface roughness measured with a proﬁlometer, given by: 2 Rq 2 −1 1.4 (21) αc,rough = αc 1 + tan π δ where αc,rough corresponds to conductor losses of a rough conductor; Rq is RMS value of the surface roughness; δ is the skin depth of the electromagnetic wave. The values of Rq measured are in the range [400, 500 nm]. The error between diﬀerent extracted Q0 factors values is indicated in the last column of Tables 2, 3 and 4. This diﬀerence can be explained by the fact that there are some loss measured in realized structures that are not taken into account in the HFSS simulation and analytical formulas as measurement errors. The Q0 factors of resonators realized with composite conductors to be characterized, Ag-aC, AgSnIn and AgSn, are also measured, and its values are shown in Table 2. The resonator realized with AgSn, with f0 = 6 GHz, is poorly engraved, hence unmeasurable. We have developed a script which relates the quality factor of a resonator with the electrical conductivity of a metal that forms the resonator by diﬀerent analytical formulas of losses cited in Section 2. We then extract the values of eﬀective electrical conductivities of composite conductors from measured values of quality factor shown in Table 5. Tables 6, 7 and 8 show the values of eﬀective electrical conductivities obtained by several analytical models of conductor loss for resonators with resonance frequencies 6, 10 and 15 GHz. The results obtained by diﬀerent analytical models are similar to each other. We observe that AgaC has a better electrical conductivity than AgSnIn and AgSn. The mean values of eﬀective electrical conductivity of all performed measurements are given in Table 9. According to these results, we can classify electrical conductivity of composite conductors characterized in this work, compared to those of pure conductors, in an ascending order like this: Sn, AgSn, AgSnIn, Au, Ag-aC, Cu, Ag.

Progress In Electromagnetics Research Letters, Vol. 60, 2016

79

Table 6. Eﬀective electrical conductivity of composite conductors, Ag-aC, AgSnIn and AgSn, extracted by matched asymptotic analytical model for λ/2 resonators with resonance frequencies 6, 10 and 15 GHz.

Composite conductors Ag-aC AgSnIn AgSn

Extracted eﬀective electrical conductivity (MS/m) f0 = 6 GHz f0 = 10 GHz f0 = 15 GHz 43.51 43.65 47.74 21.38 27.34 24.58 9.46 9.16

Table 7. Eﬀective electrical conductivity of composite conductors, Ag-aC, AgSnIn and AgSn, extracted by conformal mapping analytical model for λ/2 resonators with resonance frequencies 6, 10 and 15 GHz.

Composite conductors Ag-aC AgSnIn AgSn

Extracted eﬀective electrical conductivity (MS/m) f0 = 6 GHz f0 = 10 GHz f0 = 15 GHz 48.42 46.54 49.73 28.12 25.52 27.21 10.93 10.64

Table 8. Eﬀective electrical conductivity of composite conductors, Ag-aC, AgSnIn and AgSn, extracted by conformal mapping (G. Ghione) analytical model for λ/2 resonators with resonance frequencies 6, 10 and 15 GHz.

Composite conductors Ag-aC AgSnIn AgSn

Extracted eﬀective electrical conductivity (MS/m) f0 = 6 GHz f0 = 10 GHz f0 = 15 GHz 46.78 45.60 49.13 28.53 24.47 28.55 10.36 10.5

Table 9. Mean values of eﬀective electrical conductivity of composite conductors. Composite conductors Electrical conductivity (MS/m)

Ag-aC 46.7 ± 1

AgSnIn 25.5 ± 1.2

AgSn 9.9 ± 0.36

5. CONCLUSION A microwave characterization method of electrical conductivity of composite conductors is performed using coplanar half-wavelength resonators. Several analytical models are collected from literature to calculate losses in such structures and establish an analytical relation between conductivity and quality factor. Q0 factors values of CPW half-wavelength resonators, obtained by microwave measurement for pure conductors, are in good agreement with those obtained by analytical formulas of loss and by numerical simulations. Analytical formulas of losses are used to determine the eﬀective electrical conductivity of composite conductors that form the resonators, from their measured quality factors. The results show that Ag-aC has a better electrical conductivity than Gold (Au). AgSnIn and AgSn have a better electrical conductivity than Tin (Sn).

80

Benarabi et al.

ACKNOWLEDGMENT This work is the result of a collaborative eﬀort. The authors would like to thank RADIALL and IRIES companies that have contributed to the realization of this work. The authors wishes to express their gratitude to BPI FRANCE and to FEDER for funding this work through doctoral and post-doctoral fellowships. REFERENCES 1. Hansen, R. C. and W. T. Pawlewicz, “Eﬀective conductivity and microwave reﬂectivity of thin metallic ﬁlms,” IEEE Trans. Microwave Theory and Tech., Vol. 82, 2064–2066, Nov. 1982. 2. Maxwell, E., “Conductivity of metallic surfaces at microwave frequencies,” Applied Physics, Vol. 18, No. 2, Jul. 1947. 3. Beilenho, K., et al., “Open and short circuits in coplanar MMIC’s,” IEEE Trans. Microwave Theory and Tech., Vol. 41, No. 4, 1534–1537, Sep. 1993. 4. Holloway, C. L. and E. F. Kuester, “A quasi-closed form expression for the conductor loss of CPW lines, with an investigation of edge shape edge eﬀects,” IEEE Trans. Microwave Theory and Tech., Vol. 43, No. 6, 2695–2701, Dec. 1995. 5. Collin, R. E., Foundations for Microwave Engineering, 2nd edition, 178–179, McGraw-Hill, New York, 1992. 6. Ghione, G. and C. U. Naldi, “A new analytical, cad-oriented model for the ohmic and radiations losses of asymmetric coplanar lines in hybrid and monolithic MIC’s,” Gallium Arsenide Applications Symposium, GAAS, 1992, Noordwijk, Netherlands, Apr. 27–29, 1992. 7. Owyang, G. H. and T. Wu, “The approximate parameters of slot lines and their complement,” IRE Transactions on Antennas and Propagation, Vol. 6, No. 1, 49–55, Jan. 2003. 8. Holloway, C. L. and E. F. Kuester, “A quasi-closed form expression for the conductor loss of CPW lines, with an investigation of edge shape eﬀects,” IEEE Trans. Microwave Theory and Tech., Vol. 43, No. 12, 2695–2701, Dec. 1995. 9. Frankel, Y., et al., “Terahertz attenuation and dispersion characteristics of coplanar transmission lines,” IEEE Trans. Microwave Theory and Tech., Vol. 39, No. 1, Jun. 1991. 10. Belohoubek, E. and E. Denlinger, “Loss considerations for microstrip resonators,” IEEE Trans. Microwave Theory and Tech., Vol. 23, No. 1, 522–526, Janvier, 2003. 11. Tsang, L., X. Gu, and H. Braunisch, “Eﬀects of random rough surface on absorption by conductors at microwave frequencies,” IEEE Microwave and Wireless Components Letters, Vol. 16, No. 4, Apr. 2006.

Microwave Characterization of Electrical Conductivity of Composite Conductors by Half-Wavelength Coplanar Resonator Bilal Benarabi1, * , Faouzi Kahlouche1 , Bernard Bayard1 , Anthony Chavanne2 , and Jeremy Sautel3

Abstract—The aim of this work is to characterize the electrical conductivity of composite conductors deposited on an alumina substrate. Several half-wavelength coplanar resonators are realized using several pure conductors, silver (Ag), copper (Cu), gold (Au) and tin (Sn), to compare their quality factors (Q0 ), related to losses, with those from analytical methods. In the literature, losses in coplanar components have been estimated by diﬀerent analytical methods. We have put in evidence the relationship between electrical conductivity of the conductor and the resonator quality factor. An overall good agreement among quality factor values obtained by the analytical formulas, by numerical simulations and by microwave measurements is observed. The surface roughness is taken into account to better estimate real conductor losses. Therefore, these analytical formulas are used to extract the electrical conductivity values of the composite conductors (Ag-aC, AgSnIn and AgSn), from measured quality factors.

1. INTRODUCTION This work is part of a research project (Plug In Nano) whose objective is to oﬀer a new composite conductor, instead of gold used as a coating conductor in microwave and automotive connectors. The new composite conductors developed during this project have unknown electrical conductivities. In the literature, little work has been done on the characterization of the eﬀective electrical conductivity of materials [1, 2]. Our characterization method makes use of the relationship between the resonator quality factor (Q0 ) and associated losses (αT ), which depends, among several parameters, on the electrical conductivity of the metal which forms the resonator. Several analytical formulas for the estimation of these losses, in coplanar components (CPW), have been developed [3, 4]. First, we have veriﬁed experimentally and numerically these formulas by microwave measurements of losses and quality factor Q0 of half-wavelength resonators realized by some known conductors such as silver (Ag), copper (Cu), gold (Au) and tin (Sn). Then, we have extracted the electrical conductivities values of the composite conductors from measured quality factors of resonators realized with these metals. Three new composite conductors are measured here, which are: silveramorphous carbon (Ag-aC), silver-tin-indium (AgSnIn) and silver-tin (AgSn). 2. ANALYTICAL FORMULAS OF LOSSES Three loss sources are considered in coplanar half-wavelength (λ/2) resonator, as shown in Figure 1: - Conductor loss (αc ); because of the ﬁnite conductivity of the conductor. Received 4 March 2016, Accepted 10 April 2016, Scheduled 20 May 2016 * Corresponding author: Bilal Benarabi ([email protected]). 1 Laboratoire Hubert Curien, UMR CNRS 5516, 18 rue Benoˆ ıt Lauras, St-Etienne 42000, France. Bouth´eon Cedex, France. 3 Radiall-Centr’Alp, 642 rue E. Romanet, Voreppe 38340, France.

2

IREIS, ZI Sud, Andr´ ezieux-

74

Benarabi et al.

W

S

W

Resonant line (λ/2)

ε0 t

h

Figure 1. λ/2 CPW resonator.

ε 0 εr

Figure 2. CPW line dimensions.

- Dielectric loss (αd ); due to the heating eﬀects in the dielectric. - Radiation loss (αr ); which can be split into surface wave and space wave components. 2.1. Dielectric Loss For CPW line, the attenuation due to dielectric losses in the substrate is [5]: π εr αd = q tan δ [Np/m] √ λ0 εeﬀ

(1)

tan δ is the dielectric loss tangent and εeﬀ the eﬀective permittivity of the CPW, εeﬀ = 1 + q (εr − 1)

(2)

1 K(k1 ) K(k0 ) 2 K(k1 ) K(k0 )

(3)

q is the ﬁlling factor, q=

The terms K (k1 ) and K (k0 ) are the complete elliptic integrals of the ﬁrst kind with moduli k0 and k1 , which are given by: sinh(πS/4h) π(S + 2W ) sinh 4h S k0 = S + 2W are the complementary moduli given by 2 = 1 − k0,1 k0,1 k1 =

The terms k0,1

(4)

(5)

(6)

S, W and h are the geometric parameters of the structure (Figure 2). 2.2. Conductor Loss The attenuation constant αc due to conductor loss in the center strip conductor and the ground planes of the CPW is investigated by several methods. - In the Conformal Mapping method [5], the expression of attenuation constant αc is given below. The assumption made in deriving this expression is that thickness t of the CPW conductors is far greater than the skin depth δ in the metal. Typically, t is greater than 5δ. Rc + Rg [Np/m] (7) 2Z0 where Rc is the series resistance in ohms per unit length of the center strip conductor and is given by: 4πS Rs 1 + k0 π + ln − k0 ln (8) Rc = t 1 − k0 4S 1 − k02 K 2 (k0 ) αc =

Progress In Electromagnetics Research Letters, Vol. 60, 2016

75

Rg is the distributed series resistance in ohms per unit length of the ground planes and is given by: k0 Rs 1 + k0 4π(S + 2W ) 1 ln π + ln − (9) Rg = t k0 1 − k0 4S 1 − k02 K 2 (k0 ) and Z0 is the coplanar waveguide characteristic impedance. The term Rs is the skin eﬀect surface resistance given by: 1 Rs = [Ohms] (10) σδ where σ is the conductivity of the conductor in Siemens/meter and δ the skin depth. - Ghione and Naldi [6] obtained the expression for the conductor loss through an extension of Owyang an Wu’s conformal mapping approach [7]:

√ Rs εeﬀ 8πa(1 − k0 ) 1 8πb(1 − k0 ) 1 π + log − π + log (11) αc = a t(1 + k0 ) b t(1 + k0 ) 480πK(k0 )K (k0 ) 1 − k02 - In Matched Asymptotic technique [8], both the ﬁnite thickness and non-ideal conductivity of the CPW conductors are taken into account to calculate the conductor loss. In addition, the shape of the conductor cross-section need not be rectangular, but instead can be trapezoidal. Thus, the sides of the conductor which are normally assumed to be vertical can now be considered to be inclined at an angle θ as shown in Figure 3. In the same ﬁgure, the average center strip width and ground plane separation are indicated as 2a and 2b, respectively.

Figure 3. Coplanar waveguide conductor geometry showing the stopping distance Δ and edge proﬁle θ. The attenuation constant αc due to conductor loss is given by

1 2a (b − a) 1 2b (b − a) Rsm b2 ln + ln (12) αc = 16Z0 [K 2 (k)] (b2 − a2 ) a Δ (b + a) b Δ (b + a) where a (13) k = b cot(kc t) + csc(kc t) (14) Rsm = ωμ0 tIm kc t 2π σ −j (15) kc = λ0 ωε0 The stopping distance Δ for a given conductor thickness t, skin depth δ and edge proﬁle θ is given in Table 1 in [8]. 2.3. Radiation Loss In addition to the conductor and dielectric losses, the loss of the energy radiated in the coplanar line contributes signiﬁcantly to the total losses. It strongly depends on the frequency and geometry of the structure. For thick substrates, radiation losses are dominant because the CPW radiates much in the dielectric. The attenuation constant αrd due to radiation loss is given by [9]: π 5 1 (1 − 1/ε )2 (S + 2W )2 ε3/2 r r √ f3 (16) αrd = 3 2 2 1 + 1/εr c K (k)K(k)

76

Benarabi et al.

k = k0 given in Equation (5), and f is the frequency. Equation (16) is supposed to be valid under the conditions of geometry (Figure 2) limited by 0.1 < S/W < 10, thickness of the substrate h > 3W and wavelength λ > S + 2W . Total losses (αT ) which are the sum of all these components are related to the resonator unloaded quality factor Q0 by the following formula [10]: √ π εeﬀ Q0 = (17) λ0 αT λ0 , εeﬀ are the free space wavelength and eﬀective permittivity, respectively, which are related to the length of the cavity resonator (l) by [5]: λ0 (18) l= √ 2 εeﬀ The Q0 factor is calculated from the load quality factor QL at resonance by: Q0 = where QL =

QL 1 − 10(−LA /20)

(19)

f0 f2–3 dB − f1–3 dB

(20)

LA is the insertion loss at resonance. f0 and f1–3 dB , f2–3 dB are, respectively, the resonant frequency and the frequencies at −3 dB. 3. REALIZATION AND MEASUREMENT The components are manufactured by the following steps. The 4 µm conductor layer is obtained by electro-deposition and chemical formulation of metal on an alumina substrate (Al2 O3 ) with a relative dielectric permittivity of 9.8 and dielectric loss tangent of 10−4 . The samples are then passed to the photolithography step and etching by an etchant which depends on the metal: ferric chloride for copper, nitric acid for silver and nickel, and cyanuric acid for gold (Figure 4). Composite conductors are etched by femtosecond laser technique (Figure 5). Three λ/2 resonators have been designed and produced following the steps mentioned above, with dimensions and resonant frequencies given in Table 1.

Figure 4. Realized CPW resonators on alumina substrate with pure conductors: Ag, Cu, Au and Sn (4 µm).

Figure 5. Realized CPW resonators on alumina substrate with composite conductors, to be characterized: Ag-aC, AgSnIn and AgSn (4 µm).

Progress In Electromagnetics Research Letters, Vol. 60, 2016

77

Table 1. Dimensions of fabricated λ/2 resonators. λ/2 resonator Length (l = λ/2) Frequency (f0 )

S = 330 µm 10.6 mm 6 GHz

W = 146 µm 6.3 mm 4.2 mm 10 GHz 15 GHz

The loaded Q factor (QL ) is calculated by Equation (24) where the frequencies are determined from S12 and S21 transmission coeﬃcients measured by a vector network analyzer (VNA) through coplanar probes after calibration with an adapted kit in the frequency band [10 MHz–25 GHz]. In the HFSS software, resonators were excited through two wave ports, and an absorbing boundary condition was applied in the air box to simulate radiation losses. We used the same dielectric substrate and diﬀerent values of ﬁnite conductivity that corresponds to the pure conductors. 4. RESULTS AND DISCUSSION Tables 2, 3 and 4 show the evolution of the unloaded quality factor of resonators realized with pure conductors: silver (Ag), copper (Cu), gold (Au) and tin (Sn), as a function of their electrical conductivities, with respectively the following values: 61, 58, 41 and 9 MS/m. According to losses formulas, dielectric and radiation losses are supposed to be constant for the same design structure, and only the conductor loss changes when the metal is altered. The results show the variation of the resonator quality factor (Q0 ) as a function of the electrical conductivity of the conductor which put in evidence the relationship between these parameters. We observe an overall good correlation between the Q0 factors obtained by the analytical formulas, numerical simulation of HFSS and by microwave measurement of the three resonators with a small diﬀerence in some points where the Q0 factor of theory and numerical simulation is a bit larger than Table 2. Experimental, numerical and analytical Q0 factors values of CPW λ/2 resonators realized by pure conductors, Ag, Cu, Au and Sn, with f0 = 6 GHz. Quality factors values (Q0 ) of CPW λ/2 resonator with f0 = 6 GHz Q0 Mean value Purs Mapping Mapping Asymptotic HFSS Measured and uncertainty conductors (G. Ghione) Ag 142.99 152.03 144.13 142.58 139.95 144.33 ± 2.7 Cu 140.33 149.58 141.46 132.6 128.36 138.46 ± 4.7 Au 87.23 93.17 88.18 84.69 85.55 87.76 ± 1.9 Sn 39.53 21.8 40.06 28.45 28.01 31.57 ± 4.1 Table 3. Experimental, numerical and analytical Q0 factors values of CPW λ/2 resonators realized by pure conductors, Ag, Cu, Au and Sn, with f0 = 10 GHz. Quality factors values (Q0 ) of CPW λ/2 resonator with f0 = 10 GHz Q0 Mean value Purs Mapping Mapping Asymptotic HFSS Measured and uncertainty conductors (G. Ghione) Ag 132.28 130.81 132.63 128.3 123.15 129.34 ± 2.1 Cu 130.71 129.27 131.08 126.09 118.01 127.03 ± 2.9 Au 92.84 94.66 93.45 88.06 93.55 92.51 ± 1.47 Sn 46.95 50.38 47.47 45.03 39.98 45.96 ± 2.3

78

Benarabi et al.

Table 4. Experimental, numerical and analytical Q0 factors values of CPW λ/2 resonators realized by pure conductors, Ag, Cu, Au and Sn, with f0 = 15 GHz. Quality factors values (Q0 ) of CPW λ/2 resonator with f0 = 15 GHz Q0 Mean value Purs Mapping Mapping Asymptotic HFSS Measured and uncertainty conductors (G. Ghione) Ag 116.56 115.92 115.86 125.3 122.07 119.42 ± 2.1 Cu 115.37 114.71 114.71 115.09 113.44 114.66 ± 0.4 Au 82.68 83.06 82.69 79.56 76.41 80.88 ± 1.5 Sn 31.12 24.53 31.42 28.03 21.66 27.35 ± 2.2 Table 5. Measured Q0 factors of λ/2 resonators with f0 = 6, 10 and 15 GHz, realized by composite conductors. Composite conductors Q0 factors (f0 = 6 GHz) Q0 factors (f0 = 10 GHz) Q0 factors (f0 = 15 GHz)

Ag-aC 100.39 105.6 89.3

AgSnIn 57.94 67.92 64.95

AgSn 49.7 56.43

measured one. The surface roughness of conductors increases the conductor losses (αc ). We have used Hammerstad and Bekkadal formula [11], to take into account the eﬀects of surface roughness measured with a proﬁlometer, given by: 2 Rq 2 −1 1.4 (21) αc,rough = αc 1 + tan π δ where αc,rough corresponds to conductor losses of a rough conductor; Rq is RMS value of the surface roughness; δ is the skin depth of the electromagnetic wave. The values of Rq measured are in the range [400, 500 nm]. The error between diﬀerent extracted Q0 factors values is indicated in the last column of Tables 2, 3 and 4. This diﬀerence can be explained by the fact that there are some loss measured in realized structures that are not taken into account in the HFSS simulation and analytical formulas as measurement errors. The Q0 factors of resonators realized with composite conductors to be characterized, Ag-aC, AgSnIn and AgSn, are also measured, and its values are shown in Table 2. The resonator realized with AgSn, with f0 = 6 GHz, is poorly engraved, hence unmeasurable. We have developed a script which relates the quality factor of a resonator with the electrical conductivity of a metal that forms the resonator by diﬀerent analytical formulas of losses cited in Section 2. We then extract the values of eﬀective electrical conductivities of composite conductors from measured values of quality factor shown in Table 5. Tables 6, 7 and 8 show the values of eﬀective electrical conductivities obtained by several analytical models of conductor loss for resonators with resonance frequencies 6, 10 and 15 GHz. The results obtained by diﬀerent analytical models are similar to each other. We observe that AgaC has a better electrical conductivity than AgSnIn and AgSn. The mean values of eﬀective electrical conductivity of all performed measurements are given in Table 9. According to these results, we can classify electrical conductivity of composite conductors characterized in this work, compared to those of pure conductors, in an ascending order like this: Sn, AgSn, AgSnIn, Au, Ag-aC, Cu, Ag.

Progress In Electromagnetics Research Letters, Vol. 60, 2016

79

Table 6. Eﬀective electrical conductivity of composite conductors, Ag-aC, AgSnIn and AgSn, extracted by matched asymptotic analytical model for λ/2 resonators with resonance frequencies 6, 10 and 15 GHz.

Composite conductors Ag-aC AgSnIn AgSn

Extracted eﬀective electrical conductivity (MS/m) f0 = 6 GHz f0 = 10 GHz f0 = 15 GHz 43.51 43.65 47.74 21.38 27.34 24.58 9.46 9.16

Table 7. Eﬀective electrical conductivity of composite conductors, Ag-aC, AgSnIn and AgSn, extracted by conformal mapping analytical model for λ/2 resonators with resonance frequencies 6, 10 and 15 GHz.

Composite conductors Ag-aC AgSnIn AgSn

Extracted eﬀective electrical conductivity (MS/m) f0 = 6 GHz f0 = 10 GHz f0 = 15 GHz 48.42 46.54 49.73 28.12 25.52 27.21 10.93 10.64

Table 8. Eﬀective electrical conductivity of composite conductors, Ag-aC, AgSnIn and AgSn, extracted by conformal mapping (G. Ghione) analytical model for λ/2 resonators with resonance frequencies 6, 10 and 15 GHz.

Composite conductors Ag-aC AgSnIn AgSn

Extracted eﬀective electrical conductivity (MS/m) f0 = 6 GHz f0 = 10 GHz f0 = 15 GHz 46.78 45.60 49.13 28.53 24.47 28.55 10.36 10.5

Table 9. Mean values of eﬀective electrical conductivity of composite conductors. Composite conductors Electrical conductivity (MS/m)

Ag-aC 46.7 ± 1

AgSnIn 25.5 ± 1.2

AgSn 9.9 ± 0.36

5. CONCLUSION A microwave characterization method of electrical conductivity of composite conductors is performed using coplanar half-wavelength resonators. Several analytical models are collected from literature to calculate losses in such structures and establish an analytical relation between conductivity and quality factor. Q0 factors values of CPW half-wavelength resonators, obtained by microwave measurement for pure conductors, are in good agreement with those obtained by analytical formulas of loss and by numerical simulations. Analytical formulas of losses are used to determine the eﬀective electrical conductivity of composite conductors that form the resonators, from their measured quality factors. The results show that Ag-aC has a better electrical conductivity than Gold (Au). AgSnIn and AgSn have a better electrical conductivity than Tin (Sn).

80

Benarabi et al.

ACKNOWLEDGMENT This work is the result of a collaborative eﬀort. The authors would like to thank RADIALL and IRIES companies that have contributed to the realization of this work. The authors wishes to express their gratitude to BPI FRANCE and to FEDER for funding this work through doctoral and post-doctoral fellowships. REFERENCES 1. Hansen, R. C. and W. T. Pawlewicz, “Eﬀective conductivity and microwave reﬂectivity of thin metallic ﬁlms,” IEEE Trans. Microwave Theory and Tech., Vol. 82, 2064–2066, Nov. 1982. 2. Maxwell, E., “Conductivity of metallic surfaces at microwave frequencies,” Applied Physics, Vol. 18, No. 2, Jul. 1947. 3. Beilenho, K., et al., “Open and short circuits in coplanar MMIC’s,” IEEE Trans. Microwave Theory and Tech., Vol. 41, No. 4, 1534–1537, Sep. 1993. 4. Holloway, C. L. and E. F. Kuester, “A quasi-closed form expression for the conductor loss of CPW lines, with an investigation of edge shape edge eﬀects,” IEEE Trans. Microwave Theory and Tech., Vol. 43, No. 6, 2695–2701, Dec. 1995. 5. Collin, R. E., Foundations for Microwave Engineering, 2nd edition, 178–179, McGraw-Hill, New York, 1992. 6. Ghione, G. and C. U. Naldi, “A new analytical, cad-oriented model for the ohmic and radiations losses of asymmetric coplanar lines in hybrid and monolithic MIC’s,” Gallium Arsenide Applications Symposium, GAAS, 1992, Noordwijk, Netherlands, Apr. 27–29, 1992. 7. Owyang, G. H. and T. Wu, “The approximate parameters of slot lines and their complement,” IRE Transactions on Antennas and Propagation, Vol. 6, No. 1, 49–55, Jan. 2003. 8. Holloway, C. L. and E. F. Kuester, “A quasi-closed form expression for the conductor loss of CPW lines, with an investigation of edge shape eﬀects,” IEEE Trans. Microwave Theory and Tech., Vol. 43, No. 12, 2695–2701, Dec. 1995. 9. Frankel, Y., et al., “Terahertz attenuation and dispersion characteristics of coplanar transmission lines,” IEEE Trans. Microwave Theory and Tech., Vol. 39, No. 1, Jun. 1991. 10. Belohoubek, E. and E. Denlinger, “Loss considerations for microstrip resonators,” IEEE Trans. Microwave Theory and Tech., Vol. 23, No. 1, 522–526, Janvier, 2003. 11. Tsang, L., X. Gu, and H. Braunisch, “Eﬀects of random rough surface on absorption by conductors at microwave frequencies,” IEEE Microwave and Wireless Components Letters, Vol. 16, No. 4, Apr. 2006.